#------------------------------------------------------------------------------
#$Date: 2016-03-23 01:32:26 +0100 (Wed 23 de Mar de 2016) $
#$Revision: 179185 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/31/4313192.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4313192
loop_
_publ_author_name
'Katharine E. Stitzer'
'Ahmed El Abed'
'Mark D. Smith'
'Matthew J. Davis'
'Seung-Joo Kim'
'Jacques Darriet'
'Hans-Conrad zur Loye'
_publ_contact_author
;
 Hanno zur Loye
 University of South Carolina
 Dept. of Chemistry and Biochemistry
 Columbia, SC 29208
;
_publ_contact_author_email       ' zurloye@sc.edu '
_publ_section_title
;
 Crystal Growth of Novel Osmium-Containing Triple Perovskites
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              947
_journal_page_last               949
_journal_paper_doi               10.1021/ic026124p
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'Ba3 Na O9 Os2'
_chemical_formula_weight         959.41
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   5.88580(10)
_cell_length_b                   5.88580(10)
_cell_length_c                   14.3451(5)
_cell_measurement_reflns_used    4378
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      42.604
_cell_measurement_theta_min      2.840
_cell_volume                     430.373(18)
_computing_cell_refinement       'SAINT+ NT V6.02a (Bruker, 1998)'
_computing_data_collection       'SMART NT V5.625 (Bruker, 2000)'
_computing_data_reduction        'SAINT+ NT V6.02a'
_computing_molecular_graphics    'SHELXTL V5.1 (Sheldrick, 1997)'
_computing_publication_material  'SHELXTL V5.1'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0395
_diffrn_reflns_av_sigmaI/netI    0.0192
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            6055
_diffrn_reflns_theta_full        42.60
_diffrn_reflns_theta_max         42.60
_diffrn_reflns_theta_min         2.84
_diffrn_standards_decay_%        none
_exptl_absorpt_coefficient_mu    43.013
_exptl_absorpt_correction_T_max  0.1777
_exptl_absorpt_correction_T_min  0.0791
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS, Bruker, 1997)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.404
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       fragment
_exptl_crystal_F_000             806
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         3.299
_refine_diff_density_min         -3.780
_refine_diff_density_rms         0.416
_refine_ls_extinction_coef       0.0118(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.234
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         648
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.234
_refine_ls_R_factor_all          0.0354
_refine_ls_R_factor_gt           0.0342
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0245P)²+12.9000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0786
_refine_ls_wR_factor_ref         0.0793
_reflns_number_gt                635
_reflns_number_total             648
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic026124p-2_s1_1.cif
_cod_data_source_block           k3047bs
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4313192
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.6667 0.3333 0.08832(6) 0.01168(14) Uani 1 6 d S . .
Ba2 Ba 0.0000 0.0000 0.2500 0.00961(16) Uani 1 12 d S . .
Na1 Na 0.0000 0.0000 0.0000 0.0112(12) Uani 1 12 d S . .
Os1 Os 0.3333 0.6667 0.16115(3) 0.00608(11) Uani 1 6 d S . .
O1 O 0.1808(5) 0.3617(11) 0.0910(4) 0.0116(9) Uani 1 2 d S . .
O2 O 0.0206(16) 0.5103(8) 0.2500 0.0116(12) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Os Os -1.2165 7.6030 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Ba1 O2 64.2(2) 1_655 3 ?
O2 Ba1 O2 64.2(2) 1_655 2_665 ?
O2 Ba1 O2 64.2(2) 3 2_665 ?
O2 Ba1 O1 91.12(11) 1_655 2_655 ?
O2 Ba1 O1 56.18(15) 3 2_655 ?
O2 Ba1 O1 120.36(14) 2_665 2_655 ?
O2 Ba1 O1 56.18(15) 1_655 3_665 ?
O2 Ba1 O1 120.36(14) 3 3_665 ?
O2 Ba1 O1 91.12(11) 2_665 3_665 ?
O1 Ba1 O1 119.983(5) 2_655 3_665 ?
O2 Ba1 O1 56.18(15) 1_655 1_655 ?
O2 Ba1 O1 91.12(11) 3 1_655 ?
O2 Ba1 O1 120.36(14) 2_665 1_655 ?
O1 Ba1 O1 65.6(2) 2_655 1_655 ?
O1 Ba1 O1 54.4(2) 3_665 1_655 ?
O2 Ba1 O1 120.36(14) 1_655 3 ?
O2 Ba1 O1 56.18(15) 3 3 ?
O2 Ba1 O1 91.12(11) 2_665 3 ?
O1 Ba1 O1 54.4(2) 2_655 3 ?
O1 Ba1 O1 174.2(2) 3_665 3 ?
O1 Ba1 O1 119.983(5) 1_655 3 ?
O2 Ba1 O1 91.12(11) 1_655 2_665 ?
O2 Ba1 O1 120.36(14) 3 2_665 ?
O2 Ba1 O1 56.18(15) 2_665 2_665 ?
O1 Ba1 O1 174.2(2) 2_655 2_665 ?
O1 Ba1 O1 65.6(2) 3_665 2_665 ?
O1 Ba1 O1 119.983(5) 1_655 2_665 ?
O1 Ba1 O1 119.983(5) 3 2_665 ?
O2 Ba1 O1 120.36(14) 1_655 . ?
O2 Ba1 O1 91.12(11) 3 . ?
O2 Ba1 O1 56.18(15) 2_665 . ?
O1 Ba1 O1 119.983(5) 2_655 . ?
O1 Ba1 O1 119.983(5) 3_665 . ?
O1 Ba1 O1 174.2(2) 1_655 . ?
O1 Ba1 O1 65.6(2) 3 . ?
O1 Ba1 O1 54.4(2) 2_665 . ?
O2 Ba1 O1 121.12(13) 1_655 15_655 ?
O2 Ba1 O1 121.12(13) 3 15_655 ?
O2 Ba1 O1 173.27(16) 2_665 15_655 ?
O1 Ba1 O1 64.96(17) 2_655 15_655 ?
O1 Ba1 O1 89.20(11) 3_665 15_655 ?
O1 Ba1 O1 64.96(17) 1_655 15_655 ?
O1 Ba1 O1 89.20(11) 3 15_655 ?
O1 Ba1 O1 118.12(8) 2_665 15_655 ?
O1 Ba1 O1 118.12(8) . 15_655 ?
O2 Ba1 O1 173.27(16) 1_655 14 ?
O2 Ba1 O1 121.12(13) 3 14 ?
O2 Ba1 O1 121.12(13) 2_665 14 ?
O1 Ba1 O1 89.20(11) 2_655 14 ?
O1 Ba1 O1 118.12(8) 3_665 14 ?
O1 Ba1 O1 118.12(8) 1_655 14 ?
O1 Ba1 O1 64.96(17) 3 14 ?
O1 Ba1 O1 89.20(11) 2_665 14 ?
O1 Ba1 O1 64.96(17) . 14 ?
O1 Ba1 O1 53.21(16) 15_655 14 ?
O2 Ba1 O1 121.12(13) 1_655 13_665 ?
O2 Ba1 O1 173.27(16) 3 13_665 ?
O2 Ba1 O1 121.12(13) 2_665 13_665 ?
O1 Ba1 O1 118.12(8) 2_655 13_665 ?
O1 Ba1 O1 64.96(17) 3_665 13_665 ?
O1 Ba1 O1 89.20(11) 1_655 13_665 ?
O1 Ba1 O1 118.12(8) 3 13_665 ?
O1 Ba1 O1 64.96(17) 2_665 13_665 ?
O1 Ba1 O1 89.20(11) . 13_665 ?
O1 Ba1 O1 53.21(16) 15_655 13_665 ?
O1 Ba1 O1 53.21(16) 14 13_665 ?
O1 Ba2 O1 143.36(8) 16_556 2 ?
O1 Ba2 O1 65.98(16) 16_556 18_556 ?
O1 Ba2 O1 143.36(8) 2 18_556 ?
O1 Ba2 O1 143.36(8) 16_556 3 ?
O1 Ba2 O1 65.98(16) 2 3 ?
O1 Ba2 O1 102.1(2) 18_556 3 ?
O1 Ba2 O1 102.1(2) 16_556 . ?
O1 Ba2 O1 65.98(16) 2 . ?
O1 Ba2 O1 143.36(8) 18_556 . ?
O1 Ba2 O1 65.98(16) 3 . ?
O1 Ba2 O1 65.98(16) 16_556 17_556 ?
O1 Ba2 O1 102.1(2) 2 17_556 ?
O1 Ba2 O1 65.98(16) 18_556 17_556 ?
O1 Ba2 O1 143.36(8) 3 17_556 ?
O1 Ba2 O1 143.36(8) . 17_556 ?
O1 Ba2 O2 56.27(10) 16_556 2_665 ?
O1 Ba2 O2 122.20(10) 2 2_665 ?
O1 Ba2 O2 91.28(10) 18_556 2_665 ?
O1 Ba2 O2 91.28(10) 3 2_665 ?
O1 Ba2 O2 56.27(10) . 2_665 ?
O1 Ba2 O2 122.20(10) 17_556 2_665 ?
O1 Ba2 O2 91.28(10) 16_556 3_455 ?
O1 Ba2 O2 56.27(10) 2 3_455 ?
O1 Ba2 O2 122.20(10) 18_556 3_455 ?
O1 Ba2 O2 122.20(10) 3 3_455 ?
O1 Ba2 O2 91.28(10) . 3_455 ?
O1 Ba2 O2 56.27(10) 17_556 3_455 ?
O2 Ba2 O2 120.0 2_665 3_455 ?
O1 Ba2 O2 122.20(10) 16_556 1_545 ?
O1 Ba2 O2 91.28(10) 2 1_545 ?
O1 Ba2 O2 56.27(10) 18_556 1_545 ?
O1 Ba2 O2 56.27(10) 3 1_545 ?
O1 Ba2 O2 122.20(10) . 1_545 ?
O1 Ba2 O2 91.28(10) 17_556 1_545 ?
O2 Ba2 O2 120.000(1) 2_665 1_545 ?
O2 Ba2 O2 120.000(1) 3_455 1_545 ?
O1 Ba2 O2 122.20(10) 16_556 2 ?
O1 Ba2 O2 56.27(10) 2 2 ?
O1 Ba2 O2 91.28(10) 18_556 2 ?
O1 Ba2 O2 91.28(10) 3 2 ?
O1 Ba2 O2 122.20(10) . 2 ?
O1 Ba2 O2 56.27(10) 17_556 2 ?
O2 Ba2 O2 175.9(3) 2_665 2 ?
O2 Ba2 O2 55.9(3) 3_455 2 ?
O2 Ba2 O2 64.1(3) 1_545 2 ?
O1 Ba2 O2 56.27(10) 16_556 . ?
O1 Ba2 O2 91.28(10) 2 . ?
O1 Ba2 O2 122.20(10) 18_556 . ?
O1 Ba2 O2 122.20(10) 3 . ?
O1 Ba2 O2 56.27(10) . . ?
O1 Ba2 O2 91.28(10) 17_556 . ?
O2 Ba2 O2 55.9(3) 2_665 . ?
O2 Ba2 O2 64.1(3) 3_455 . ?
O2 Ba2 O2 175.9(3) 1_545 . ?
O2 Ba2 O2 120.0 2 . ?
O1 Ba2 O2 91.28(10) 16_556 3 ?
O1 Ba2 O2 122.20(10) 2 3 ?
O1 Ba2 O2 56.27(10) 18_556 3 ?
O1 Ba2 O2 56.27(10) 3 3 ?
O1 Ba2 O2 91.28(10) . 3 ?
O1 Ba2 O2 122.20(10) 17_556 3 ?
O2 Ba2 O2 64.1(3) 2_665 3 ?
O2 Ba2 O2 175.9(3) 3_455 3 ?
O2 Ba2 O2 55.9(3) 1_545 3 ?
O2 Ba2 O2 120.000(1) 2 3 ?
O2 Ba2 O2 120.000(2) . 3 ?
O1 Na1 O1 180.0(3) . 13 ?
O1 Na1 O1 89.93(19) . 3 ?
O1 Na1 O1 90.07(19) 13 3 ?
O1 Na1 O1 89.93(19) . 2 ?
O1 Na1 O1 90.07(19) 13 2 ?
O1 Na1 O1 89.93(19) 3 2 ?
O1 Na1 O1 90.07(19) . 14 ?
O1 Na1 O1 89.93(19) 13 14 ?
O1 Na1 O1 90.07(19) 3 14 ?
O1 Na1 O1 180.0(2) 2 14 ?
O1 Na1 O1 90.07(19) . 15 ?
O1 Na1 O1 89.93(19) 13 15 ?
O1 Na1 O1 180.0(2) 3 15 ?
O1 Na1 O1 90.07(19) 2 15 ?
O1 Na1 O1 89.93(19) 14 15 ?
O1 Na1 Ba2 54.68(14) . . ?
O1 Na1 Ba2 125.32(14) 13 . ?
O1 Na1 Ba2 54.68(14) 3 . ?
O1 Na1 Ba2 54.68(14) 2 . ?
O1 Na1 Ba2 125.32(14) 14 . ?
O1 Na1 Ba2 125.32(14) 15 . ?
O1 Na1 Ba2 125.32(14) . 13 ?
O1 Na1 Ba2 54.68(14) 13 13 ?
O1 Na1 Ba2 125.32(14) 3 13 ?
O1 Na1 Ba2 125.32(14) 2 13 ?
O1 Na1 Ba2 54.68(14) 14 13 ?
O1 Na1 Ba2 54.68(14) 15 13 ?
Ba2 Na1 Ba2 180.0 . 13 ?
O1 Na1 Ba1 54.251(6) . 1_455 ?
O1 Na1 Ba1 125.749(6) 13 1_455 ?
O1 Na1 Ba1 124.24(14) 3 1_455 ?
O1 Na1 Ba1 54.251(6) 2 1_455 ?
O1 Na1 Ba1 125.749(6) 14 1_455 ?
O1 Na1 Ba1 55.76(14) 15 1_455 ?
Ba2 Na1 Ba1 69.553(12) . 1_455 ?
Ba2 Na1 Ba1 110.447(12) 13 1_455 ?
O1 Na1 Ba1 125.749(6) . 13_655 ?
O1 Na1 Ba1 54.251(6) 13 13_655 ?
O1 Na1 Ba1 55.76(14) 3 13_655 ?
O1 Na1 Ba1 125.749(6) 2 13_655 ?
O1 Na1 Ba1 54.251(6) 14 13_655 ?
O1 Na1 Ba1 124.24(14) 15 13_655 ?
Ba2 Na1 Ba1 110.447(12) . 13_655 ?
Ba2 Na1 Ba1 69.553(12) 13 13_655 ?
Ba1 Na1 Ba1 180.00(2) 1_455 13_655 ?
O1 Na1 Ba1 125.749(6) . 13 ?
O1 Na1 Ba1 54.251(6) 13 13 ?
O1 Na1 Ba1 125.749(6) 3 13 ?
O1 Na1 Ba1 55.76(14) 2 13 ?
O1 Na1 Ba1 124.24(14) 14 13 ?
O1 Na1 Ba1 54.251(6) 15 13 ?
Ba2 Na1 Ba1 110.447(12) . 13 ?
Ba2 Na1 Ba1 69.553(12) 13 13 ?
Ba1 Na1 Ba1 71.522(12) 1_455 13 ?
Ba1 Na1 Ba1 108.478(12) 13_655 13 ?
O1 Na1 Ba1 54.251(6) . . ?
O1 Na1 Ba1 125.749(6) 13 . ?
O1 Na1 Ba1 54.251(6) 3 . ?
O1 Na1 Ba1 124.24(14) 2 . ?
O1 Na1 Ba1 55.76(14) 14 . ?
O1 Na1 Ba1 125.749(6) 15 . ?
Ba2 Na1 Ba1 69.553(12) . . ?
Ba2 Na1 Ba1 110.447(12) 13 . ?
Ba1 Na1 Ba1 108.478(12) 1_455 . ?
Ba1 Na1 Ba1 71.522(12) 13_655 . ?
Ba1 Na1 Ba1 180.00(2) 13 . ?
O1 Os1 O1 93.3(2) 3_565 . ?
O1 Os1 O1 93.3(2) 3_565 2_665 ?
O1 Os1 O1 93.3(2) . 2_665 ?
O1 Os1 O2 90.64(16) 3_565 3_565 ?
O1 Os1 O2 174.3(2) . 3_565 ?
O1 Os1 O2 90.64(16) 2_665 3_565 ?
O1 Os1 O2 90.64(16) 3_565 . ?
O1 Os1 O2 90.64(16) . . ?
O1 Os1 O2 174.3(2) 2_665 . ?
O2 Os1 O2 85.1(2) 3_565 . ?
O1 Os1 O2 174.3(2) 3_565 2_665 ?
O1 Os1 O2 90.64(16) . 2_665 ?
O1 Os1 O2 90.64(16) 2_665 2_665 ?
O2 Os1 O2 85.1(2) 3_565 2_665 ?
O2 Os1 O2 85.1(2) . 2_665 ?
O1 Os1 Os1 122.90(17) 3_565 16_556 ?
O1 Os1 Os1 122.90(17) . 16_556 ?
O1 Os1 Os1 122.90(17) 2_665 16_556 ?
O2 Os1 Os1 51.36(15) 3_565 16_556 ?
O2 Os1 Os1 51.36(15) . 16_556 ?
O2 Os1 Os1 51.36(14) 2_665 16_556 ?
O1 Os1 Ba1 55.882(8) 3_565 1_455 ?
O1 Os1 Ba1 55.882(7) . 1_455 ?
O1 Os1 Ba1 130.01(17) 2_665 1_455 ?
O2 Os1 Ba1 123.835(14) 3_565 1_455 ?
O2 Os1 Ba1 55.73(15) . 1_455 ?
O2 Os1 Ba1 123.835(15) 2_665 1_455 ?
Os1 Os1 Ba1 107.090(14) 16_556 1_455 ?
O1 Os1 Ba1 55.882(8) 3_565 1_565 ?
O1 Os1 Ba1 130.01(17) . 1_565 ?
O1 Os1 Ba1 55.882(7) 2_665 1_565 ?
O2 Os1 Ba1 55.73(15) 3_565 1_565 ?
O2 Os1 Ba1 123.835(15) . 1_565 ?
O2 Os1 Ba1 123.835(15) 2_665 1_565 ?
Os1 Os1 Ba1 107.090(14) 16_556 1_565 ?
Ba1 Os1 Ba1 111.744(13) 1_455 1_565 ?
O1 Os1 Ba1 130.01(17) 3_565 . ?
O1 Os1 Ba1 55.882(7) . . ?
O1 Os1 Ba1 55.882(7) 2_665 . ?
O2 Os1 Ba1 123.835(15) 3_565 . ?
O2 Os1 Ba1 123.835(15) . . ?
O2 Os1 Ba1 55.73(14) 2_665 . ?
Os1 Os1 Ba1 107.090(14) 16_556 . ?
Ba1 Os1 Ba1 111.744(13) 1_455 . ?
Ba1 Os1 Ba1 111.744(13) 1_565 . ?
O1 Os1 Ba1 57.10(17) 3_565 13_665 ?
O1 Os1 Ba1 57.10(17) . 13_665 ?
O1 Os1 Ba1 57.10(17) 2_665 13_665 ?
O2 Os1 Ba1 128.64(15) 3_565 13_665 ?
O2 Os1 Ba1 128.64(15) . 13_665 ?
O2 Os1 Ba1 128.64(14) 2_665 13_665 ?
Os1 Os1 Ba1 180.0 16_556 13_665 ?
Ba1 Os1 Ba1 72.910(14) 1_455 13_665 ?
Ba1 Os1 Ba1 72.910(14) 1_565 13_665 ?
Ba1 Os1 Ba1 72.910(14) . 13_665 ?
O1 Os1 Ba2 53.46(17) 3_565 1_565 ?
O1 Os1 Ba2 125.720(9) . 1_565 ?
O1 Os1 Ba2 125.720(9) 2_665 1_565 ?
O2 Os1 Ba2 54.201(5) 3_565 1_565 ?
O2 Os1 Ba2 54.201(5) . 1_565 ?
O2 Os1 Ba2 120.80(14) 2_665 1_565 ?
Os1 Os1 Ba2 69.441(6) 16_556 1_565 ?
Ba1 Os1 Ba2 69.862(6) 1_455 1_565 ?
Ba1 Os1 Ba2 69.862(6) 1_565 1_565 ?
Ba1 Os1 Ba2 176.531(18) . 1_565 ?
Ba1 Os1 Ba2 110.559(6) 13_665 1_565 ?
Os1 O1 Na1 177.6(3) . . ?
Os1 O1 Ba2 96.1(2) . . ?
Na1 O1 Ba2 86.36(17) . . ?
Os1 O1 Ba1 92.77(10) . 1_455 ?
Na1 O1 Ba1 87.27(10) . 1_455 ?
Ba2 O1 Ba1 88.83(11) . 1_455 ?
Os1 O1 Ba1 92.77(10) . . ?
Na1 O1 Ba1 87.27(10) . . ?
Ba2 O1 Ba1 88.83(11) . . ?
Ba1 O1 Ba1 174.2(2) 1_455 . ?
Os1 O1 Ba1 91.8(2) . 13_665 ?
Na1 O1 Ba1 85.82(16) . 13_665 ?
Ba2 O1 Ba1 172.2(2) . 13_665 ?
Ba1 O1 Ba1 90.80(11) 1_455 13_665 ?
Ba1 O1 Ba1 90.80(11) . 13_665 ?
Os1 O2 Os1 77.3(3) 16_556 . ?
Os1 O2 Ba1 166.5(3) 16_556 1_455 ?
Os1 O2 Ba1 89.23(2) . 1_455 ?
Os1 O2 Ba1 89.23(2) 16_556 16_456 ?
Os1 O2 Ba1 166.5(3) . 16_456 ?
Ba1 O2 Ba1 104.2(3) 1_455 16_456 ?
Os1 O2 Ba2 91.59(12) 16_556 1_565 ?
Os1 O2 Ba2 91.59(12) . 1_565 ?
Ba1 O2 Ba2 88.75(10) 1_455 1_565 ?
Ba1 O2 Ba2 88.75(10) 16_456 1_565 ?
Os1 O2 Ba2 91.59(12) 16_556 . ?
Os1 O2 Ba2 91.59(12) . . ?
Ba1 O2 Ba2 88.75(10) 1_455 . ?
Ba1 O2 Ba2 88.75(10) 16_456 . ?
Ba2 O2 Ba2 175.9(3) 1_565 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 O2 2.938(5) 1_655 ?
Ba1 O2 2.938(5) 3 ?
Ba1 O2 2.938(5) 2_665 ?
Ba1 O1 2.9467(3) 2_655 ?
Ba1 O1 2.9467(3) 3_665 ?
Ba1 O1 2.9467(3) 1_655 ?
Ba1 O1 2.9467(3) 3 ?
Ba1 O1 2.9467(3) 2_665 ?
Ba1 O1 2.9467(3) . ?
Ba1 O1 3.006(5) 15_655 ?
Ba1 O1 3.006(5) 14 ?
Ba1 O1 3.006(5) 13_665 ?
Ba2 O1 2.932(5) 16_556 ?
Ba2 O1 2.932(5) 2 ?
Ba2 O1 2.932(5) 18_556 ?
Ba2 O1 2.932(5) 3 ?
Ba2 O1 2.932(5) . ?
Ba2 O1 2.932(5) 17_556 ?
Ba2 O2 2.9448(3) 2_665 ?
Ba2 O2 2.9448(3) 3_455 ?
Ba2 O2 2.9448(3) 1_545 ?
Ba2 O2 2.9448(3) 2 ?
Ba2 O2 2.9448(3) . ?
Ba2 O2 2.9448(3) 3 ?
Na1 O1 2.259(5) . ?
Na1 O1 2.259(5) 13 ?
Na1 O1 2.259(5) 3 ?
Na1 O1 2.259(5) 2 ?
Na1 O1 2.259(5) 14 ?
Na1 O1 2.259(5) 15 ?
Na1 Ba2 3.58627(13) 13 ?
Na1 Ba1 3.6267(3) 1_455 ?
Na1 Ba1 3.6267(3) 13_655 ?
Na1 Ba1 3.6267(3) 13 ?
Os1 O1 1.852(5) 3_565 ?
Os1 O1 1.852(5) . ?
Os1 O1 1.852(5) 2_665 ?
Os1 O2 2.041(6) 3_565 ?
Os1 O2 2.041(6) . ?
Os1 O2 2.041(6) 2_665 ?
Os1 Os1 2.5490(8) 16_556 ?
Os1 Ba1 3.5552(3) 1_455 ?
Os1 Ba1 3.5552(3) 1_565 ?
Os1 Ba1 3.5787(9) 13_665 ?
Os1 Ba2 3.62932(15) 1_565 ?
O1 Ba1 2.9467(3) 1_455 ?
O1 Ba1 3.006(5) 13_665 ?
O2 Os1 2.041(6) 16_556 ?
O2 Ba1 2.938(5) 1_455 ?
O2 Ba1 2.938(5) 16_456 ?
O2 Ba2 2.9448(3) 1_565 ?
